Presentation on theme: "Organic Solar Cells Greg Smestad (http://www.solideas.com/solrcell/cellkit.html) developed this experiment.http://www.solideas.com/solrcell/cellkit.html."— Presentation transcript:
Organic Solar Cells Greg Smestad (http://www.solideas.com/solrcell/cellkit.html) developed this experiment.http://www.solideas.com/solrcell/cellkit.html
Goal In the past year the price of fossil fuels has increased more than anytime in recent memory. Because of this fact, the race for alternate energy sources to replace or lessen the use of fossil fuels has risen. This activity of creating electricity through the use of organic solar cells is an example of one way scientists are trying to alleviate some of the dependence on non- renewable resources. It is the purpose of this activity for students to see that with a little human ingenuity, other ways to create energy can be attained.
Safety In the initial stages of this lab, when using the powered TiO 2 care should be taken not to inhale this compound. Massing, grinding, and heating should be done in a fume hood or a well ventilated area. If this is not possible, a ventilation mask should be worn. Goggles and gloves are also recommended throughout the lab.
Procedure Prepare the TiO 2 Suspension In 1 mL increments, add 9 mL of very dilute acetic acid solution (0.1 mL concentrated acetic acid to 50 mL of distilled or deionized water.) to 6 g of TiO 2 powder in a mortar and pestle while grinding. The grinding process mechanically separates the aggregated TiO 2 particles due to the high shear forces generated. Add each 1 mL addition of the dilute acid solution only when the previous mixing and grinding has produced a uniform and lump-free suspension with a consistency of a thick paint. The grinding process requires about 30 minutes and should be done in a well-ventilated area. (a Fume hood if you have one)
Procedure Prepare the TiO 2 Suspension To the TiO 2 paste, add a drop of Triton X or two drops of clear dish washing detergent, and swirl. This allows the final suspension to more uniformly coat the glass plates. So as not to produce foam, the TiO 2 suspension should not be ground or agitated after the surfactant is added. Transfer half of the TiO 2 suspension in to each of the 2 provided small dropper bottles and allow it to equilibrate for at least 15 minutes (if not overnight) for best results. These bottles will need to be shared with the entire class.
Procedure Preparation of the TiO 2 slide Obtain 2 glass plates and clean with ethanol. Do not touch the faces of the plates once they are cleaned! Determine which side of each glass plate is conducting with a multimeter (set it to measure resistance). Put the glass plates side by side with one conducting side up and one conducting side down. Cover 1mm of each long edge of the plates with Scotch tape. Cover 4-5 mm of the short edge of the conductive side up with Scotch tape. Add 2 drops of the white TiO 2 solution on the conductive side up glass. Quickly spread the white TiO 2 solution evenly with a glass pipette, sweeping first away from the second slide, then sweeping the extra TiO 2 onto the second glass slide.
Procedure Preparation of the TiO 2 slide Obtain 2 glass plates and clean with ethanol. Do not touch the faces of the plates once they are cleaned! Determine which side of each glass plate is conducting with a multimeter (set it to measure resistance). Put the glass plates side by side with one conducting side up and one conducting side down. (A) Cover 1mm of each long edge of the plates with Scotch tape. (set it to measure resistance). (set it to measure resistance). (B) Cover 4-5 mm of the short edge of the conductive side up with Scotch tape. (C) Add 2 drops of the white TiO 2 solution on the conductive side up glass. (D) Quickly spread the white TiO 2 solution evenly with a glass pipette, sweeping first away from the second slide, then sweeping the extra TiO 2 onto the second glass slide. (E)
Procedure Preparation of the TiO 2 slide Remove the tape and place the TiO 2 -coated glass on the hot plate, keeping track of where your plate is. Clean the TiO 2 from the other glass plate with ethanol and save it for the next part of the lab. Heat the glass on a hotplate turned to high in a hood for 10-20 minutes. The surface turns brown as the organic solvent and surfactant dries and burns off to produce a white or green titanium dioxide coating.(Note: this requires a plate that gets quite hot.) Allow the glass to slowly cool by turning off the hotplate.
Procedure Staining the TiO 2 slide Crush fresh or frozen raspberries, blackberries, pomegranate seeds, bing cherries, or red Hibiscus tea into a Petri dish. Pour part of the crushed berries into a coffee filter and with gloves on squeeze the bottom of the filter so the juice goes into the Petri dish. There should be enough juice in the Petri dish to cover the TiO 2 slide when placed face down to soak.
Procedure Staining the TiO 2 slide Soak the slide (face down) for 10 minutes in this liquid to stain the slide to a deep red- purple color. If the slide is not uniformly stained, then put it back in the liquid for 5 more minutes. Wash the slide first with distilled water then ethanol and gently blot it dry with a tissue. While the TiO 2 slide is soaking in the liquid, use this time to prepare the graphite slide. (Do not remove the TiO 2 slide from the liquid until you have finished the graphite slide.)
Procedure Preparation of the graphite slide Pass the other slide of tin oxide glass, conducting side down, through a candle flame to coat the conducting side with carbon (soot). For best results, pass the glass piece quickly and repeatedly through the middle part of the flame. Wipe off the carbon along the perimeter of three sides of the carbon- coated glass plate using a cotton swab.
Procedure Assembling the Solar Cell Place the carbon-coated glass plate face down on the TiO 2 -coated glass plate. The two glass plates must be slightly offset (5 mm). Hold the plates together with binder clips on each side of the longer edges. Add 2 drops of the iodide solution on an offset side and allow it to soak through. Alternately open and close each side of the solar cell by releasing and returning the binder clips to help the iodide solution move through. Make sure that all of the stained area is contacted by the iodide solution. Wipe off excess iodide solution on the exposed area (important) with tissue paper.
Procedure Assembling the Solar Cell Connect a multimeter using an alligator clip to each plate (the negative electrode is the TiO 2 coated glass and the positive electrode is the carbon coated glass). Make sure the light is shining through the TiO 2 coated glass first. Test the current and voltage produced by solar illumination, or an overhead projector.
Data Using your readings from the multimeter complete the following table. GroupOverhead Projector Off Overhead Projector On Sunlight Voltage (V) Current (mA) Voltage (V) Current (mA) Voltage (V) Current (mA) 1. 2. 3. 4. Average
Solar Cell Mechanism Dye Molecule – absorbs a photon of light, exciting an electron from its ground-state orbital into an excited-state orbital, making it easy for the electron to come free from the molecule and travel through the electrical circuit TiO 2 Nanocrystals – are very small, so they have a high surface area. When annealed (cooked) they fuse to form a very rough (and therefore very large) surface area. The dye molecules react with this surface, forming bonds so that they can stick to it. The larger the surface area, the more dye molecules can be attached to the surface and therefore the more electrons can be excited at any given time. The TiO 2 is a semi-conductor, so it enables the electrons to move away (conduct) from the dye molecules and into the circuit Electrodes – conduct the electrons from the cell into the electrical circuit. This allows the electrons to flow through the circuit (in our case, a multimeter). Flowing electrons are called electricity! Tin oxide (SnO 2 ) coated glass is used because it is both conductive and transparent, and we want light to pass through the electrodes into the solar cell. Electrolyte – when the dye loses an electron, it becomes positively charged, and needs obtain another electron to be re-neutralized. (It will then be able to react again when another photon comes along!) The iodide ion (I – ) is able to provide the required electron, thereby neutralizing both the iodide and the dye molecule. Iodine is not stable as a single neutral atom, so two neutral atoms of iodine react with an additional iodide ion to form triiodide (I 3 – ). Carbon – Recall that electrons are flowing OUT through the TiO 2 -coated electrode and IN through the carbon-coated electrode. The carbon acts as a catalyst, allowing two incoming electrons to react with one molecule of triiodide to form three iodide ions, thus completing the cycle.